Please copy and paste this embed script to where you want to embed

Problem Set # 3 Solution ECEN 3320 Fall 2013 Semiconductor Devices September 9, 2013 – Due September 18, 2013 1. A semiconductor has Eg = 1.40 eV and m∗h = 0.5m0 ; m∗e = 0.1m0 at T = 300◦ K. (a) Calculate the position of the intrinsic Fermi level, Ef , with respect to the middle of the band gap, Ei − Emidgap = Ei − Eg /2. Solution: The intrinsic Fermi level is defined in terms of the bandgap, temperature and effective carried masses as 3 m∗h Ec − Ev = kT ln . 2 4 m∗e

Ei −

Using the given values, we find that the distance of the Fermi level from the center of the gap is Ei −

Ec − Ev 3 = 0.0258 ln(5) = 0.750.02581.61 ≈ 0.0313eV 2 4

(b) Calculate the intrinsic carrier concentration, ni . Solution: The intrinsic carrier concentration in terms of the effective densities of states, Nc and Nv and the bandgap energy as ni =

p

Nc Nv exp [−Eg /kT ] .

Recalling that the effecive densities of states are given by m∗e kT 3/2 = 2 2π¯h2 ∗ mh kT 3/2 = 2 2π¯h2

Nc Nv

we find that for a bare electron m0 kT N0 = 2 2π¯h2

3/2

= 2.61 × 1019 cm−3 .

Using the above, we find that ni ≈ (0.05)3/2 2.61 × 1019 × exp(−0.70/0.0258) ≈ 4.8 × 106 cm−3 . 1

(c) Impurity atoms are added so that the Fermi level, Ef , is 0.35 eV above the middle of the band gap. i. Are the impurities donors or acceptors? Solution: The impurities are donors as donors raise the Fermi level. The intrinsic Fermi level is raised by only 0.03 eV relative to the center of gap. The ’measured’ 0.35 eV is much larger than this indicating the semiconductor is an extrinsic ndoped semiconductor. ii. What was the concentration of impurities added? Solution: We need to make an additional assumption here, the assumption that the donor impurities are shallow. It is only the shallow impurities (within a few kT of the band edge) that will contribute to the repositioning of the Fermi level relative to the intrinsic Fermi level. Ef − Ei ND = n0 = ni exp kT

that evaluates to ND ≈ 1.07 × 1012 cm−3 . 2. Determine the equilibrium electron and hole concentrations in silicon for the following conditions. Solution: Using the fact that there is no free charge density in an equilibrium material, we can write that n0 − p0 + Na− − Nd+ = 0. The law of mass action n0 p0 = n2i combined with the above gives that n20 + (Na+ − Nd− )n0 − n2i = 0 p20 + (Nd− − Na+ )p0 − n2i = 0 with solutions (omitting the spurious one generated by multiplying through by n0 (p0 )), we find Nd−

n0 =

Na+

p0 =

− 2

Na+

− 2

Nd−

!

v ! u u N − − Na+ 2 t d + + n2

2

!

i

v ! u u Na+ − N − 2 t d + + n2

2

i

These relations can generally be simplified significantly. For an intrinsic semiconductor, Nd+ ni and Na− ni and, therefore, n0 ≈ ni + (Nd+ − Na− ) and p0 ≈ ni − (Nd+ − Na− ). For an extrinsic semiconductor, for example, an n-type, ni Nd+ and n0 ≈ Nd+ with p0 = n0 /n2i . In our present case, the intrinsic carrier concentration is given by ni =

εg Nc Nv exp − 2kT

p

2

≈ 1 × 1010 cm−3 .

We see that in all cases, except (d), below, |Nd − Na | ni and, therefore, the semiconductors are extrinsic. For extrinsic, non-degenerate seminconductors, we can equate the majority concentration with the difference |Nd − Na | and calculate the minority concentration from the law of mass action that n2i = n0 p0 . When the semiconductor is so lightly doped that it remains intrinsic, we can simply subtract the doping concentration from the intrinsic (see (d) below). (a) T = 300◦ K, Nd = 2 × 1015 cm−3 , Na = 0. Solution: We have that n0 ≈ Nd − Na = 2 × 1015 cm−3 and therefore p0 ≈

n2i ≈ 5 × 104 cm−3 n0

(b) T = 300◦ K,Nd = 0, Na = 1 × 1016 cm−3 . Solution: We have that p0 ≈ Na − Nd = 1 × 1016 cm−3 and therefore n0 ≈

n2i ≈ ×104 cm−3 p0

(c) T = 300◦ K, Nd+ = 2 × 1015 cm−3 , Na = 1 × 1015 cm−3 . Solution: We have that n0 ≈ Nd+ − Na− = 1. × 1015 cm−3 and therefore p0 ≈

n2i ≈ ×105 cm−3 n0

(d) T = 300◦ K, Nd+ = 1 × 109 cm−3 , Na− = 0. Solution: Here we have n0 ≈ 1.1 × 1010 cm−3 p0 ≈ 9.9 × 109 cm−3 (e) T = 500◦ K, Nd+ = 1 × 1014 cm−3 , Na− = 0. h

ε −ε

i

Solution: At T = 500◦ C, the ni = Nc exp ckT f ≈ 8.53 × 1013 cm−3 . We need to use the general form to find the n0 and p0 . Writing v u

N + − Na+ u Nd+ − Na+ n0 = d +t 2 2

!2

+ n2i ≈ 1.49 × 1014 cm−3 .

we therefore find that p0 ≈

n2i ≈ 4.89 × 1013 cm−3 . n0 3

3. (a) If Ec − Ef = 0.2eV in GaAs at T = 500◦ K, calculate the values of the equilibrium carrier concentrations, n and p. Solution: The equilibrium carrier concentrations are given by "

#

Ec − Ef n = Nc (T = 500 C) exp − = 9.05 × 1015 cm−3 . kT |T =500◦ C ◦

The band gap of GaAs at room temperature is roughly 1.424 eV. As Ec −Ef = 0.2eV, then Ef − Ev = 1.224eV and we can evaluate

p = Nv exp −

Ec − Ef = 7.56 × 106 cm−3 . kT

(b) Assuming that the value of n you obtained in (a) remains constant, calculate Ec − Ef and p at T = 300◦ K. Solution: We have n Ec − Ef = −kT ln . Nc

Plugging in n = 9.05 × 1015 Ec − Ef = −kT ln Nc (500◦ C)

!

≈ 0.1eV.

The value of Ef − Ev should now be circa 1.324 eV. Evaluating

p = Nv exp −

Ef − Ev kT

≈ 4.40 × 10−4 cm−3 .

4. A certain semiconductor is doped with Nd = 2 × 1013 cm−3 and NA = 0. The intrinisic carrier concentration for this semiconductor is ni = 2 × 1013 cm−3 . (a) Determine the majority and minority carrier concentrations at thermal equilibrium. Solution: Here, we have that Nd+ ≈ ni so we must use the general solution for concentration in terms of doping to find the effective concentrations. Writing

n0 =

Nd+

− 2

Na+

v ! u u N + − Na+ 2 d +t + n2i ≈ 3 × 1013 cm−3 .

2

(b) Determine the position of the energy level relative to the intrinsic Fermi level, Ef − Ei . Solution: We have that

Ef − Ei = kT ln

4

n ni

≈ 0.01eV

View more...
Ei −

Using the given values, we find that the distance of the Fermi level from the center of the gap is Ei −

Ec − Ev 3 = 0.0258 ln(5) = 0.750.02581.61 ≈ 0.0313eV 2 4

(b) Calculate the intrinsic carrier concentration, ni . Solution: The intrinsic carrier concentration in terms of the effective densities of states, Nc and Nv and the bandgap energy as ni =

p

Nc Nv exp [−Eg /kT ] .

Recalling that the effecive densities of states are given by m∗e kT 3/2 = 2 2π¯h2 ∗ mh kT 3/2 = 2 2π¯h2

Nc Nv

we find that for a bare electron m0 kT N0 = 2 2π¯h2

3/2

= 2.61 × 1019 cm−3 .

Using the above, we find that ni ≈ (0.05)3/2 2.61 × 1019 × exp(−0.70/0.0258) ≈ 4.8 × 106 cm−3 . 1

(c) Impurity atoms are added so that the Fermi level, Ef , is 0.35 eV above the middle of the band gap. i. Are the impurities donors or acceptors? Solution: The impurities are donors as donors raise the Fermi level. The intrinsic Fermi level is raised by only 0.03 eV relative to the center of gap. The ’measured’ 0.35 eV is much larger than this indicating the semiconductor is an extrinsic ndoped semiconductor. ii. What was the concentration of impurities added? Solution: We need to make an additional assumption here, the assumption that the donor impurities are shallow. It is only the shallow impurities (within a few kT of the band edge) that will contribute to the repositioning of the Fermi level relative to the intrinsic Fermi level. Ef − Ei ND = n0 = ni exp kT

that evaluates to ND ≈ 1.07 × 1012 cm−3 . 2. Determine the equilibrium electron and hole concentrations in silicon for the following conditions. Solution: Using the fact that there is no free charge density in an equilibrium material, we can write that n0 − p0 + Na− − Nd+ = 0. The law of mass action n0 p0 = n2i combined with the above gives that n20 + (Na+ − Nd− )n0 − n2i = 0 p20 + (Nd− − Na+ )p0 − n2i = 0 with solutions (omitting the spurious one generated by multiplying through by n0 (p0 )), we find Nd−

n0 =

Na+

p0 =

− 2

Na+

− 2

Nd−

!

v ! u u N − − Na+ 2 t d + + n2

2

!

i

v ! u u Na+ − N − 2 t d + + n2

2

i

These relations can generally be simplified significantly. For an intrinsic semiconductor, Nd+ ni and Na− ni and, therefore, n0 ≈ ni + (Nd+ − Na− ) and p0 ≈ ni − (Nd+ − Na− ). For an extrinsic semiconductor, for example, an n-type, ni Nd+ and n0 ≈ Nd+ with p0 = n0 /n2i . In our present case, the intrinsic carrier concentration is given by ni =

εg Nc Nv exp − 2kT

p

2

≈ 1 × 1010 cm−3 .

We see that in all cases, except (d), below, |Nd − Na | ni and, therefore, the semiconductors are extrinsic. For extrinsic, non-degenerate seminconductors, we can equate the majority concentration with the difference |Nd − Na | and calculate the minority concentration from the law of mass action that n2i = n0 p0 . When the semiconductor is so lightly doped that it remains intrinsic, we can simply subtract the doping concentration from the intrinsic (see (d) below). (a) T = 300◦ K, Nd = 2 × 1015 cm−3 , Na = 0. Solution: We have that n0 ≈ Nd − Na = 2 × 1015 cm−3 and therefore p0 ≈

n2i ≈ 5 × 104 cm−3 n0

(b) T = 300◦ K,Nd = 0, Na = 1 × 1016 cm−3 . Solution: We have that p0 ≈ Na − Nd = 1 × 1016 cm−3 and therefore n0 ≈

n2i ≈ ×104 cm−3 p0

(c) T = 300◦ K, Nd+ = 2 × 1015 cm−3 , Na = 1 × 1015 cm−3 . Solution: We have that n0 ≈ Nd+ − Na− = 1. × 1015 cm−3 and therefore p0 ≈

n2i ≈ ×105 cm−3 n0

(d) T = 300◦ K, Nd+ = 1 × 109 cm−3 , Na− = 0. Solution: Here we have n0 ≈ 1.1 × 1010 cm−3 p0 ≈ 9.9 × 109 cm−3 (e) T = 500◦ K, Nd+ = 1 × 1014 cm−3 , Na− = 0. h

ε −ε

i

Solution: At T = 500◦ C, the ni = Nc exp ckT f ≈ 8.53 × 1013 cm−3 . We need to use the general form to find the n0 and p0 . Writing v u

N + − Na+ u Nd+ − Na+ n0 = d +t 2 2

!2

+ n2i ≈ 1.49 × 1014 cm−3 .

we therefore find that p0 ≈

n2i ≈ 4.89 × 1013 cm−3 . n0 3

3. (a) If Ec − Ef = 0.2eV in GaAs at T = 500◦ K, calculate the values of the equilibrium carrier concentrations, n and p. Solution: The equilibrium carrier concentrations are given by "

#

Ec − Ef n = Nc (T = 500 C) exp − = 9.05 × 1015 cm−3 . kT |T =500◦ C ◦

The band gap of GaAs at room temperature is roughly 1.424 eV. As Ec −Ef = 0.2eV, then Ef − Ev = 1.224eV and we can evaluate

p = Nv exp −

Ec − Ef = 7.56 × 106 cm−3 . kT

(b) Assuming that the value of n you obtained in (a) remains constant, calculate Ec − Ef and p at T = 300◦ K. Solution: We have n Ec − Ef = −kT ln . Nc

Plugging in n = 9.05 × 1015 Ec − Ef = −kT ln Nc (500◦ C)

!

≈ 0.1eV.

The value of Ef − Ev should now be circa 1.324 eV. Evaluating

p = Nv exp −

Ef − Ev kT

≈ 4.40 × 10−4 cm−3 .

4. A certain semiconductor is doped with Nd = 2 × 1013 cm−3 and NA = 0. The intrinisic carrier concentration for this semiconductor is ni = 2 × 1013 cm−3 . (a) Determine the majority and minority carrier concentrations at thermal equilibrium. Solution: Here, we have that Nd+ ≈ ni so we must use the general solution for concentration in terms of doping to find the effective concentrations. Writing

n0 =

Nd+

− 2

Na+

v ! u u N + − Na+ 2 d +t + n2i ≈ 3 × 1013 cm−3 .

2

(b) Determine the position of the energy level relative to the intrinsic Fermi level, Ef − Ei . Solution: We have that

Ef − Ei = kT ln

4

n ni

≈ 0.01eV

Thank you for interesting in our services. We are a non-profit group that run this website to share documents. We need your help to maintenance this website.